Author
others
View
4
Download
0
Embed Size (px)
Strength and Stiffness Properties of the Optimum Mix Composition of Cement-less Wastepaper-based Lightweight Block (CWLB)
OKEYINKA ORIYOMI M, OLOKE DAVID A, KHATIB JAMAL M
School of Architecture and the Built Environment
Faculty of Science and Engineering
University of Wolverhampton, City Campus,
Wolverhampton, West Midlands WV1 1SB,
UNITED KINGDOM
Abstract: - The cement-less wastepaper-based lightweight block (CWLB) is a newly developed eco-friendly
non-load bearing block manufactured from majorly cellulosic wastes without the use of cement. The main
constituents of CWLB includes; wastepaper aggregate (WPA) produced from post-consumer wastepaper, waste
additive and sand. This study was conducted to determine its optimum mix composition and the corresponding
strength and stiffness properties. The experimentations carried out covered; the optimization of the mix
composition of CWLB using the Taguchi statistical optimization technique (TSOT) and the determination of
the compressive strength, density, elastic modulus and the ultrasonic pulse velocity (UPV) of the optimal
CWLB specimen. The findings from the TSOT ascertains that the optimum mix composition of CWLB
comprises of processing parameters including; 2.5 WPA/sand ratio, 0.75 water/binder ratio, and 3.5 Metric ton
(i.e. 13.7 MPa) compacting force. Also, it was found that the optimal CWLB exhibited; an average compressive
strength of 2.71 MPa, an average density of 901.5 kg/m3, an average UPV of 989.9 m/s and an estimated elastic
modulus of 883.4 MPa. The comparison of these properties with the applicable standard requirements indicates
the suitability of CWLB for non-load bearing application. In addition, the presence of 75% waste content in the
mix composition of CWLB indicates its eco-friendliness and its potential to contribute to the sustainability in
the construction industry through reduction in natural resources consumption. The innovation presented in this
study includes; the development of a suitable optimum mix composition of constituent materials for the novel
CWLB, the identification of factors that affects it strength properties and the determination of its engineering
properties. Future work will investigate other relevant properties of CWLB which include; capillary water
absorption, thermal conductivity, and the reaction to fire.
Key-Words: - Taguchi method, compressive strength, non -loadbearing, block, Wastepaper, Mix composition,
Optimization, Density, Ultrasonic pulse velocity (UPV), Elastic modulus.
1 Introduction The various notable environmental impacts
associated with the creation of the built environment
and the unsustainable waste generation resulting
from increased civilization and proliferating
standard of living represents major issues of global
environmental concerns. Critical analysis of the
Municipal Solid Waste (MSW) generation growth
from 0.64 kg/day in 2002 to 1.2 kg/day in 2012 [1]
suggests that the world experienced an estimated
88% increase in per capital MSW generation within
a ten years period. The construction industry on the
other hand is reported to be responsible for 60% raw
material consumption at the global level [2]. A
typical evidence of this impact is the fact that; the
building industry requires about six to seven more
tonnes of sand and gravel, for each single tonne of
cement used in construction [3] aside from the
excessive raw materials being exhausted in cement
production [4].
Following the continuous suggestion and
consideration for the use of environmental friendly
materials, minimization of raw material
consumption [5], practice of industrial ecology [5],
and the attempts of researchers to achieve
sustainability in the construction industry through
recycled use of waste in the production of
construction materials [6], building materials such
as: fibre cement board [7], lightweight block [8];
[9]; [10], low density board [11], papercrete [10];
[8], plastering mortar [12], have been produced
from wastepaper. However, extensive literature
review showed that, building material produced
from waste paper suffers high water absorption [8;
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 335 Volume 13, 2017
13; 12] thickness swelling and low strength with
increasing wastepaper fibre content [8]; [14]; [15];
[16]. This drawback of strength reduction arises due
to the corresponding water content increment that
occurs in the mix with increasing wastepaper
content [17]. This implies that contradiction exists
between the hygroscopic properties of paper fibre
and the moderate water requirement for cement
hydration and it means that the high water/cement
ratio resulting from increasing paper content lowers
the strength of the building material concerned.
Aside this, the utilization of considerable quantity of
cement in the composition of wastepaper based
building materials as a means of strength properties
improvement is believed to be undermining their
environmental friendliness.
Thus, the development of cement-less wastepaper-
based lightweight block (CWLB) is another
important step towards the production of eco-
friendly building materials from wastepaper. This
block which was designed to be used for non-load
bearing/non-structural application was developed
without the use of hydraulic cement. Its constituents
are majorly waste materials, which includes;
wastepaper aggregate (WPA), waste additive
(obtained as industrial waste by-product), and lesser
quantities of sand, water and natural admixture.
CWLB was specifically developed to address the
low compressive strength which usually occurs with
increasing waste paper content in wastepaper based
blocks produced with cement as binding medium.
Having developed the mixture proportioning
process [18] and identified the; Water/binder ratio,
WPA/sand ratio, and compacting force as the crucial
factors that affects the compressive strength of
CWLB [19], this study was conducted to determine
the optimum mix composition of CWLB (using the
Taguchi statistical optimization technique) and also
determine the strength and stiffness properties of the
specimen produced from same. The essence is to
obtain the maximized compressive strength of
CWLB and assess its suitability for use in wall
construction with reference to the standard
requirements for non-loadbearing blocks. The
corresponding UPV and the elastic modulus of the
optimal CWLB specimen were also determined to
assess its quality and stiffness.
1.1 Structure of the Study The studies presented in this paper are divided into
two major categories. The first study category dealt
with the optimization of the mix composition of
CWLB using the Taguchi statistical optimization
technique. The experimental and the analytical
details for the optimization study are presented in
section 2.1 to s.1.2 of this paper. The second study
category dealt with the determination of the strength
and stiffness properties (including: compressive
strength, density, UPV and elastic modulus) of the
resulting optimal CWLB, the experimental details
are presented in 2.2 of this paper. The findings from
the optimization study are presented in section 3.1
to 3.3.1 and the findings from the investigated
properties are presented in section 3.3.2 to 3.3.4.
The conclusion of the studies and the future work in
progress are presented in section 4 of this paper.
1.2 Taguchi Method The Taguchi method is a statistical optimization
process technique developed by Genichi Taguchi
around the 1950s [20]. It is a design of experiment
DOE [21] approach that is grounded on quality
philosophy which seeks to develop product and
processes that are robust to environmental factors
and other sources of variation. Robustness can be
described as the extent of the product or processes
capabilities to perform efficiently and consistently
with minimal effect from the uncontrollable noise
factors due to operation or manufacturing [21].
The use of Taguchi approach in product
development offers design engineer a proficient and
an organised means of determining a near optimum
design parameters for quality performance. The
concept of signal-to-noise-ratio encompassed within
the Taguchi method enables the measurement of
variability of performance response relative to the
desired value under different noise conditions.
Taguchi method recognises that in product
development, some factors that cause variability can
be controlled while there are also factors that are
uncontrollable. The uncontrollable factors are
known as noise factors. The identification of
controllable factors is important in Taguchi DOE,
because, during experimentation, noise factors are
controlled to force variability to occur thereby
leading to the determination of optimal control
factors setting that make the process or product
robust or resistant to variation from the noise
factors. The noise factors are regarded as the cause
of variability in performance as well as product
failure. The S/N ratio helps to evaluate the stability
of performance of an output characteristic [22].
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 336 Volume 13, 2017
Fig. 1: Procedure for Taguchi design methodology [22]
2 Materials and Methods In this study, CWLB was produced from constituent
materials which includes; wastepaper aggregate
(WPA), sand, waste additives (binder), natural
admixture (stoneware clay) and water. The WPA
utilized as major aggregate filler was systematically
produced from post-consumer wastepaper (old
newsprint), the detail procedure is reported in [19].
The waste additive used as binder was obtained as a
byproduct of food processing industry, its elemental
composition is presented in Table (1). The sand
utilized as minor additional filler and the stoneware
clay utilized as admixture were obtained from local
suppliers in Wolverhampton, United Kingdom.
Given the variation in the physical properties of the
constituent materials (Table 2), batching was carried
out by weight in order to achieve accurate
proportioning of materials for the CWLB mixes.
Several mixes were prepared from varied
combinations of WPA/sand ratios, WPA/binder
ratios, and water/binder ratios. CWLB specimens of
sizes 50mm x 50mm x50mm were molded using a
10 ton manual hydraulic press containing a
preinstalled pressure gauge (Fig. 2).
Table 1: Elemental Composition of the Waste Additive Utilised as Binder
Elements Waste additive Solid part Liquid part ppm ppm
Al 0.03 0.01
Ca 5.42 6.09
Fe 0.08 0.02
K 6.60 28.87
Mg 0.40 3.06
S 0.78 2.15
Si 65.71 27.20
Table 2: Physical Properties of Constituent Materials of CWLB
Phys
ical
Pro
pert
ies
Materials
Was
tepa
per
Agg
rega
te (W
PA)
Sand
Was
te A
dditi
ve
(bin
der)
Nat
ural
adm
ixtu
re
(Sto
new
are
clay
)
Specific gravity
0.66
1
2.63
1.04 0.895
Loose Bulk density (kg/l)
0.09
6
1.428 0.911
Part
icle
si
zes r
ange
(m
m)
(3 -
0.1
25
)
(4 -
0.0
63
)
Not
appli
cable
< 0
.063
Perc
enta
ge
Solid
co
nten
t (%
)
10
0
10
0
23
10
0
The CWLB specimens produced from all laboratory
experimentation in this study were cured in ambient
laboratory air for 28 days duration prior to testing.
The first part of this study dealt with the
optimisation of CWLB while the second part
determines the strength and stiffness properties of
the optimal CWLB specimen. Each of the tests were
conducted on three samples of CWLB cubic
specimens.
10 Perform a confirmatory experiment and implement results
9. Perform statistical analysis
8. Conduct experiments
7. Choose appropriate orthogonal array
5. Determine levels
4. Classify design parameters
3. Select quality characteristic
2. Select design or process parameters
1. Problem recognition and formulation
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 337 Volume 13, 2017
Fig. 2: 10 ton manual hydraulic press containing a preinstalled pressure gauge and CWLB Molding process
2.1 Experimental Details for the Optimisation of Mix Composition of CWLB This study employs Taguchi method to determine
the best combination of processing
parameters/control factors required to obtain the
optimum mix composition for CWLB. The
previously performed series of trial
experimentations and salient parameter studies [19]
have addressed the step 1-4 of the procedure for
Taguchi design methodology (Fig. 1). Thus, the
compressive strength of the block was solely studied
as the quality response in this optimisation process
because of its intrinsic importance in the design of
masonry structures. The Taguchi approach was
chosen over the other types of DOE (including; full
factorial, screening experiments, response surface
and mixture experiment) as it is capable of
analysing more factors with fewer experimental runs
while also enabling the analysis of effects on
response.
The optimisation experiment was designed based on
three controllable three-level processing parameters
namely; WPA/sand ratios, water/binder ratios and
compacting forces. Other processing parameters of
CWLB which includes; WPA particle size (passing
3.35 mm BS sieve size), specimen curing duration
(28 days), mixing time (27 min), admixture quantity
(5% by weight of WPA), were kept constant. The
selected processing parameters and their levels are
shown in Table 3.
With three factors, each with three levels, the full
factorial design would have required 33=27 possible
combinations of trials. Meanwhile, carrying out a
large number of experiments for all the
combinations would have amounted to excessive
resources and time consumption.
Table 3: CWLB processing parameters and levels
Des
igna
tions
Con
trol
Fa
ctor
s
Uni
ts
Lev
el 1
Lev
el 2
L
evel
3
A WPA/sand
ratio
- 2.08 2.27 2.5
B Water/binder
ratio
- 0.75 2.25 3.75
C Compacting
force
Metric
ton
3 3.25 3.5
However, the Taguchi method employed in this
study utilizes an ‘orthogonal array (OA)’ (which is
an arrangement of numbers in columns and rows in
a manner that each column represent a factor while
the rows stand for levels of the factors [23]) to
simplify the large number of experiments, and
allocates them into a smaller number of trials to run
the experiment. This explains the reason why only
three processing parameters, each with three levels,
were considered in this study. Thus, nine trials of
CWLB specimen with varied compositions were
produced using the L9 (33) OA, as presented in
Table 4a and 4b.
The 50mm x 50mm x 50mm CWLB specimen (Fig.
3) produced from the experimental runs in Table 4b
were tested for density (based on BS EN 772-
13:2011 [25]) and compressive strength (based on
BS EN 772-1:2011 [26]) after curing. Being the
focused quality response, the result of compressive
strength obtained was analysed by adopting the (the
bigger the better) signal-to-noise (S/N) ratio and by
analysis of variance (ANOVA) in order to
determine the optimal processing parameter
required to produce CWLB with satisfactory
compressive strength and to establish the impacts of
each processing parameter on the compressive
strength of CWLB.
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 338 Volume 13, 2017
Table 4a: Table of Taguchi Orthogonal Array L9 (source: Ref. [24])
Experiment
Number
Factors and level Parameter
setting
A B C
1 1 1 1 A1B1C1
2 1 2 2 A1B2C2
3 1 3 3 A1B3C3
4 2 1 2 A2B1C2
5 2 2 3 A2B2C3
6 2 3 1 A2B3C1
7 3 1 3 A3B1C3
8 3 2 1 A3B2C1
9 3 3 2 A3B3C2
Table 4b: Table of Taguchi Orthogonal Array L9(33) showing details of CWLB parameter combinations
Exper
imen
t
Num
ber
Factors and level Parameter
setting
A B C
1 1(2.08) 1(0.75) 1(3) A1B1C1
2 1(2.08) 2(2.25) 2(3.25) A1B2C2
3 1(2.08) 3(3.75) 3(3.5) A1B3C3
4 2(2.27) 1(0.75) 2(3.25) A2B1C2
5 2(2.27) 2(2.25) 3(3.5) A2B2C3
6 2(2.27) 3(3.75) 1(3) A2B3C1
7 3(2.5) 1(0.75) 3(3.5) A3B1C3
8 3(2.5) 2(2.25) 1(3) A3B2C1
9 3(2.5) 3(3.75) 2(3.25) A3B3C2
Fig. 3: 50mmx50mmx50mm CWLB specimen
2.1.1 Analysis method In analysing the results, the (S/N) ratio introduced
by Taguchi for determining product quality
characteristics was adopted. In Taguchi method, a
high S/N ratio implies that the signal is much higher
than the random effect of the noise factors. The part
or process operation consistent with the highest S/N
ratios always yields optimal quality characteristics
with minimum variance. Also, quality
characteristics in the Taguchi method can be
categorized into; ‘the smaller the better’ (indicating
minimization), ‘the nominal the better’ (indicating
nominalization) and ‘the bigger the better’
(indicating maximization) [22]. In the study of the
mechanical properties, especially compressive
strength of blocks, higher strength is usually
desired. Therefore, since the focus of this study was
to maximize the compressive strength of CWLB, the
S/N ratio which corresponds to ‘the bigger the
better’ quality characteristic was utilized in the
analysis, and it was calculated using Eqn. (1) [22]:
𝑺 𝑵𝑳⁄ = −𝟏𝟎𝒍𝒐𝒈 (𝟏
𝒏∑
𝟏
𝒚𝒊𝟐
𝒏
𝒊=𝟏) (1)
Where: 𝑦𝑖 is the value of the compressive strength
for the ith trials, n is the numbers of samples, and
𝑆 𝑁𝐿⁄ is the symbol representing ‘the bigger the
better’ signal-to-noise-ratio.
In this analysis, the level of the factor with the
larger S/N ratio denotes that this level can result in a
larger compressive strength. By selecting the level
with a larger S/N ratio for each factor, the
estimation of the set of optimal levels of the
processing parameters for CWLB was actualized. A
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 339 Volume 13, 2017
confirmation test/selection of optimum parameter
setting according to the identified optimal factor
levels was carried out as applicable. The
experimental results as well as the computed 𝑆 𝑁𝐿⁄
ratios for each parameter settings are presented in
Table 5.
2.1.2 Determination of mean of 𝑆 𝑁𝐿⁄ ratio, Main effect of control factors and the rank of effect. The averaged effect response for 𝑆 𝑁𝐿⁄ ratio of each
factor was investigated to determine the
contributions of WPA/sand ratio, Water/binder
ratio, and Compacting force to the magnitude of the
compressive strength. The Minitab 17 statistical
software was used to carry out analysis of variance
(ANOVA) on the experimental results and the
corresponding computed 𝑆 𝑁𝐿⁄ ratio and was also
use to obtain the main effect plot for 𝑆 𝑁𝐿⁄ ratio.
The mean of 𝑆 𝑁𝐿⁄ ratio j ̅𝑖 (which represented the
factor average effect at each level) was obtained by
applying the expression for determining average of
S/N ratio for each factor [24] as shown in Eqn. (2).
The effect of each factor 𝐸𝑗 (which is simply the
observed range of S/N ratio at different factor
levels) was obtained by using the expression [24]
shown in Eqn. (3). The rank was estimated based on
the magnitude of the effect of each factor.
j ̅𝒊
=𝟏
𝒏∑ 𝒋𝒊
𝒏 𝒋𝒊=𝟏 |∀𝒋,𝒊 (2)
Where:
j represents any of the factors A, B or C (at any
instance), i stands for any of the levels 1, 2 or 3 (at
any instance), j ̅𝑖 is the mean of S/N ratio, n is the
number of levels in the experiment. The sign |∀𝑗,𝑖
signifies that Eqn. (2) was evaluated at j and i
values.
𝑬𝒋 = 𝑭𝒋𝒎𝒂𝒙 − 𝑭𝒋𝒎𝒊𝒏|∀𝒊 (3)
Where:
𝐸𝑗 is the effect of factor j, 𝐹𝑗𝑚𝑎𝑥 and 𝐹𝑗𝑚𝑖𝑛 are
maximum and minimum value of factor j
respectively. The sign |∀𝑖 indicates that Eqn. (3) was
evaluated across the level.
2.2 Experimental Details for Determination of the Strength and Stiffness Properties of CWLB The tests conducted on CWLB’s optimum mix
composition (i.e. optimal CWLB specimen) to
determine its strength and stiffness properties
includes; compressive strength test (in accordance
with the BS EN 772-1:2011) [26], ultrasonic pulse
velocity (UPV) (in accordance with BS EN 12504-
4:2004 recommended procedure) [27] and elastic
modulus (estimated using Eqn. (4) which was
derived based on the principle of ultrasonic pulse
velocity testing described by BS 1881-203:1986
[28] and BS 12504-4:2004 in conjunction with the
Newton-Laplace acoustic theory).
𝑬 = 𝝆𝑽𝟐 (4)
Where; E is the elastic modulus in (MPa), ρ is the
density in (kg) and V is the UPV of the CWLB
specimen in (m/s).
3 Results and discussions The plot of compressive strength test result for each
experimental run is presented in Figure 4. It was
observed that experiment number 7 displayed the
highest compressive strength compared to all other
experimental runs. Also, the CWLB produced from
experiment number 6 displayed the lowest
compressive strength compared to others, which
indicates that parameter combination in experiment
number 6 is the worst parameter setting compared to
others.
Fig. 4: Plot of compressive strength test result for each CWLB experimental run 3.1 Main Effect of Processing Parameter/Control Factors In this study, the average compressive strength
result of CWLB samples (n=3) produced from each
experimental run was statistically analysed using
𝑆 𝑁𝐿⁄ ratio which correspond to the “bigger the
better” quality characteristics and were computed
0
0.5
1
1.5
2
2.5
3
1 2 3 4 5 6 7 8 9
Co
mp
ress
ive
str
en
gth
(M
Pa)
Experiment numbers
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 340 Volume 13, 2017
based on Equation (1), since the higher compressive
strength is desired. The computed 𝑆 𝑁𝐿⁄ ratios for
each parameter combinations are presented in Table
5.
Figure 5 present the graph of main effect plot for
𝑆 𝑁𝐿⁄ ratio which was plotted to find the optimum
levels of WPA/Sand ratio, Water/binder ratio and
compacting force required to produce CWLB with
maximal compressive strength. It was found that, an
increment in WPA/sand ratio lead to an increase in
compressive strength of the block, while a decrease
in WPA/Sand ratio resulted in a decrease in
compressive strength. However, an insignificant
effect variation was observed within the range
investigated. Low water/binder ratio resulted in
higher compressive strength while high water/binder
ratio lead to lower compressive strength and the
effect variation was significant within the range
tested. Also, the compressive strength of CWLB
increases with increasing compacting force and
decreases at lower compacting forces.
Table 5: Experimental Results and Computed 𝑺 𝑵𝑳⁄ ratio
Exp
erim
ent
Num
ber
Factors and levels
Response 𝑺 𝑵𝑳⁄ ratio
A B C Compressive strength (MPa)
1 1 1 1 1.7 4.609
2 1 2 2 0.81 -1.830
3 1 3 3 0.71 -2.975
4 2 1 2 2.10 6.444
5 2 2 3 0.96 -0.356
6 2 3 1 0.50 -6.021
7 3 1 3 2.71 8.659
8 3 2 1 0.86 -1.310
9 3 3 2 0.53 -5.514
Fig. 5: Main effect plot for WPA/ sand ratio, Water/Binder ratio, and Compacting force. 3.2 Optimum Mixture Composition of CWLB Judging from both Figure 5 and the data presented
in Table 6, the most significant processing
parameters for CWLB is factor B (Water/Binder
ratio) as it displayed the largest effect and ranked
1st. Factor A (WPA/Sand ratio) is the least
significant as it exhibited the least effect, hence
ranked 3rd. Factor C (Compacting Force) has the
second largest effect as it ranked 2nd. Furthermore,
from Table 6, the optimal parameter setting based
on maximum values was deduced to be A3B1C3
which revealed that the CWLB should be produced
from a combination of 2.5 WPA/Sand ratio, 0.75
Water/Binder ratio and 3.5 Metric ton Compacting
force. This optimal parameter setting is equivalent
to a mix ratio of 1:0.4:0.2 of WPA, Sand, and
Binder ratio.
Table 6: Mean of S/N Response, Effects of Factors and Rank of Effects
Description Factors and levels
A B C
j ̅𝑖
(see Eqn. 2)
Level 1 -0.06 6.57 -0.91
Level 2 0.02 -0.3 -0.3
Level 3 0.61 -4.84 1.78
Ej
(see Eqn. 3)
Effect 0.67 11.41 2.69
Rank of
effect
Rank 3 1 2
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 341 Volume 13, 2017
It is also equivalent to 62.5% WPA, 25% Sand and
12.5% binder when estimated based on aggregate
and binder only (i.e. excluding water content and
natural admixture).
3.3 Properties and Optimal Parameter Combination for CWLB This section evaluates the effectiveness of the
Taguchi DOE technique in optimizing the mix
composition of CWLB and discusses the
compressive strength, UPV and the elastic modulus
of the resulting optimal CWLB. Table 7 shows the
comparison of the worst and the optimal
composition of CWLB. Table 8 presents the
properties of the resulting optimal CWLB.
Table 7: Confirmation test, Properties and Optimal parameter combination for CWLB
Factors and levels
Com
pres
sive
st
reng
th (M
PA)
𝑆 𝑁𝐿⁄
ratio
A B C
Worst
compositio
n
1 3 1 0.50 -5.352
Optimal
compositio
n
3 1 3 2.71 8.659
Percentage increase 442% -
3.3.1 Confirmation Test and Review of Effectiveness of Taguchi DOE on Optimization of CWLB. Incidentally, the identified optimal parameter setting
of CWLB coincided with the parameter setting on
experiment number 7 (see Table 5). Therefore, the
result of compressive strength for experiment
number 7 was compared with the result obtained
from the worst parameter setting (i.e. experiment
number 6). From Table 7, it was established that the
optimum parameter setting increases the
compressive strength of CWLB by 442% compared
to that of the worst parameter setting. This finding
indicate the suitability of the Taguchi Method in
optimizing the mix composition of CWLB.
Table 8: Properties and Optimal parameter combination for CWLB
Properties and Optimal parameter combination for CWLB
Optimal Parameter Combination
Properties
WPA
/San
d ra
tio
Wat
er/B
inde
r ra
tio
Com
pact
ing
forc
e (M
etri
c to
n)
Com
pres
sive
st
reng
th (M
Pa)
Den
sity
(kg/
m3 )
UPV
(m/s)
Ela
stic
Mod
ulus
(M
Pa)
2.5
0.7
5
3.5
2.71 901.5 989.9 883.4
3.3.2 Compressive strength and Density of of the Optimal CWLB Specimen. As shown Table 7, the optimal CWLB exhibited an
average compressive strength of 2.71 MPa and
average density of 901.5 kg/m3. In contrast with
standard recommended mechanical and physical
property requirement for non-load bearing blocks;
the 2.71 MPa average compressive strength of
CWLB is maximally higher than the 1.5MPa
minimum compressive strength recommended by
BS EN 771-4:2011 [29] for non-load bearing
lightweight block (see Fig. 6) and the 901.5 kg/m3
average density of CWLB falls within the range of
300-1000kg/m3 (BS EN 771-4:2011) [29] and
625kg/m3-1500kg/m3 (BS EN 2028 1975) [30]
specified for lightweight non-load bearing blocks. This finding thus indicates the suitability of CWLB
for non-load bearing application in wall
construction.
In contrast with the existing cement based
wastepaper blocks (e.g. papercrete) (Fig. 6), the 2.71
MPa compressive strength displayed by CWLB is
higher than the 1.84 MPa [9] reported for papercrete
block containing 40% by volume paper pulp, and
the ≈1.4MPa [8] reported for papercrete block
containing 35.7% cement 35.7 sand and 28.6%
wastepaper (i.e. mix ratio 1: 1:0.8).
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 342 Volume 13, 2017
Fig. 6: Comparison of the compressive strength Optimized CWLB with Worst CWLB, Standard Non- load bearing block and Papercrete blocks
3.3.3 Ultrasonic pulse velocity of the Optimal CWLB The UPV of CWLB was determined using a Pundit
Ultrasonic testing equipment which consisted of; an
electronic circuit that generate pulses, a 50kHz
transducer that transforms electronic pulse into
mechanical pulse and a pulse reception circuit
which receives the signal. The UPV was calculated
from the path length (0.05m for CWLB specimen)
divided by the transit time. At optimum mix
composition, CWLB displayed an average
ultrasonic pulse velocity of 989.9m/s. The UPV of a
building material indicates its quality in terms of
strength and porosity. It should however be noted
that, there are no existing classification of UPV
values for neither wastepaper based building
materials nor masonry blocks. Evaluating the
quality of CWLB with reference to the UPV
concrete classification, the 989.9 m/s average UPV
value displayed by CWLB is comparatively less
than the 2000 m/s UPV value specified for weak
concrete. This finding thus indicates the high
porosity of CWLB microstructure and its low
strength property compared to concrete. The low
UPV value displayed by CWLB is expected,
because; it is a lightweight block and not a concrete,
and it is made from combination of cellulosic waste,
sand and non- hydraulic binder. Therefore, the
implementation of CWLB in building construction
is recommended to be limited to application as non-
load bearing lightweight blocks.
3.3.4 Elastic Modulus of the Optimal CWLB The Modulus of elasticity of a building material is
an indication for its stiffness against deformation.
For a masonry structure design to adequately
comply with serviceability specification, the
knowledge of elastic modulus of the masonry unit is
required for determination of elastic deformation
due to first application of load and for estimating
creep arising from sustained load [31].
As shown in Table 8, the elastic modulus for the
optimal CWLB specimens was estimated to be
883.4 MPa. In contrast with the existing cement-
based wastepaper block, the 883.4MPa estimated
elastic modulus for CWLB is maximally higher than
the; 800 psi (5.52 MPa), 700psi (4.83 MPa), 590 psi
(4.07 MPa) reported by [10] and [32] for papercrete
produced from paper-cement-sand of; 1:1:5 gal,
1:1:10 gal and 1:1:15 gal respectively. This finding
indicates the high stiffness characteristics of CWLB
and its suitability for use as non-load bearing
blocks.
4 Conclusions The details of the optimization of the mixture
composition of CWLB using Taguchi approach and
the investigation of the strength and stiffness
properties of the resulting optimal CWLB is
presented in this paper. CWLB specimens of sizes
50mm x 50mm x 50mm were molded from mixture
of WPA, sand, waste additive (binder), natural
admixture and water. The control parameters which
include; WPA/Sand ratio, Water/Binder ratio and
Compacting force were investigated with the aim of
maximizing the 28 days compressive strength of
CWLB. The outcome of the investigation showed
that the compressive strength of CWLB depends on
the processing parameters. Comparison of the main
effect of WPA/Sand ratio, Water/Binder ratio and
Compacting Force indicated that the Water/Binder
ratio has the most significant effect on the
compressive strength of CWLB. The identified
optimal parameter settings; 2.5 WPA/Sand ratio,
0.75 Water/Binder ratio, and 3.5 Metric ton
Compacting force produced CWLB specimen with
properties suitable for non-load bearing application
in wall construction (viz: 2.71 MPa average
compressive strength and 901.5 kg/m3 average
density, 989.9 m/s average UPV, and 883.4 MPa
0.5
2.71
1.5
1.84
1.4
0
0.5
1
1.5
2
2.5
3C
ompr
essiv
e st
reng
th(M
Pa)
Worst CWLB, Optimized CWLB, Recommended Strength and
Papercrete blocks
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 343 Volume 13, 2017
estimated elastic modulus). The optimum mix
composition of CWLB which contains; 62.5%
WPA, 25% Sand and 12.5% waste additive (binder)
makes a highly eco-friendly block as it amounts to
the presence of 75% waste content. The innovation
presented in this paper thus includes; the
development of an optimum mix composition for
the novel CWLB which provides information on the
mix ratio of the constituent material of same for
research repeatability and subsequent, the
identification of factors that affects its strength
properties along with determination of the
engineering properties of the resulting optimal
CWLB which ascertains its suitability for the
intended application. In order to take the subjected
matter further, future research will investigate the;
capillary water absorption, reaction to fire and the
thermal conductivity of CWLB.
References:
[1] Hoornweg, Daniel; Bhada-Tata, Perinaz. 2012.
What a Waste: A Global Review of Solid Waste
Management. World Bank, Washington, DC. ©
World Bank. Available at:
https://openknowledge.worldbank.org/handle/10
986/17388
[2] Hawken, Paul., Lovins, Amory B.,
Lovins,L.Hunter, (1999) Natural capitalism :
creating the next industrial revolution. [online]
Boston: Little, Brown and Co.
[3] U.S. Geological Survey (USGS), (2013) “Sand
and gravel (construction) statistics”, in: Kelly,
T.D., Matos, G.R., (Eds.), Historical statistics
for mineral and material commodities in the
United States. U.S. Geological Survey Data
Series 140, Reston
[4] Oss, H.G. and Padovani, A.C. (2003) Cement
manufacture and the environment part II:
environmental challenges and opportunities.
Journal of Industrial Ecology, 7(1), pp. 93-126.
[5] Mehta, P.K., (2002) Greening of the Concrete
Industry for Sustainable Development. ACI
Concrete International, 24(7): pp. 23-28.
[6] Okeyinka Oriyomi M., Oloke David A., Khatib
Jamal M., (2015a) A Review on Recycled Use
of Solid Wastes in Building Materials.
International Journal of Civil, Environmental,
Structural, Construction and Architectural
Engineering, Vol: 9, No:12. Available at:
http://waset.org/publications/10003128/a-
review-on-recycled-use-of-solid-wastes-in-
building-materials
[7] Ashori, A., Tabarsa, T. and Valizadeh, I. (2011)
Fiber reinforced cement boards made from
recycled newsprint paper. Materials Science
and Engineering, [online], 528(25), pp. 7801-
7804.
[8] Akinwumi, I.I., Olatunbosun, O.M., Olofinnade,
O.M. and Awoyera, P.O. (2014) Structural
Evaluation of Lightweight Concrete Produced
Using Waste Newspaper and Office Paper. Civil
and Environmental Research [online], 6(7), pp.
160-167.
[9] Modry,S. (2001) Use of Waste Paper as a
Constituent of Concrete. Recovery and
recycling of paper international symposium,
Thomas Telford Publishing, United Kingdom.
pp.77-80.
[10] Fuller,B., Fafitis,A. and Santamaria,J.
(2006) Structural Properties of a New Material
Made of Waste Paper AEI 2006: Building
Integration Solutions. ASCE, pp.1-16.
[11] Esmeralda, Y. A. O.; Marcos, A. E. S.;
Mario Rabelo S.; Utilization of wastepaper to
manufacture low density boards. Bioresource
Technology, 2000, 73, 77 –79.
[12] Aciu, C., Iluţiu–Varvara, D.A., Cobirzan, N.
and Balog, A. (2014) Recycling of paper waste
in the composition of plastering mortars.
Procedia Technology [online], 12pp. 295-300
[13] Titzman, L.C. (2006) Analysis of low-cost
building material for the MixAlco process.
Master's thesis, Texas A&M
University.Available electronically from
http://hdl.handle.net/1969 [online].
[14] Okeyinka Oriyomi M. and Idowu
Oluwatobi J. (2014) Assessment of the
Suitability of Paper Waste as an Engineering
Material. Engineering, Technology & Applied
Science Research, Vol. 4, No. 6, pp. 724-727
[15] Decard J. D.; West R. P.; Prichard S. J
(2001)The impact response of recycled paper
waste concrete. In : Ravindra Dhir K., Mukesh
C. Limbachiya Ed., Proceedings of the
International symposium on recovery and
recycling of paper ,United Kingdom, 2001,81-
92
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 344 Volume 13, 2017
[16] Yun,H., Jung,H. and Choi,C. (2007)
Mechanical properties of papercrete containing
waste paper . 18th International Conference on
Composite Materials. [online].
[17] Mohamad Shukeri, R., Ghani, A. and Naser,
A. (2008) Concrete Mix With Wastepaper. 2nd
International Conference On Built Environment
In Developing Countries (ICBEDC 2008).
[online]. Available at:
http://eprints.usm.my/25137/1/BUILDING_EN
GINEERING_AND_CONSTRUCTION_6.pdf
[18] Okeyinka O.M., David D.A, Jamal Khatib.
(2015b). Development of Environmentally
Friendly Light weight block from Waste paper.
2nd International Sustainable Buildings
Symposium (ISBS 2015), 28-30 May, Gazi
University, Ankara –Turkiye. 406-416.
Available At:
<http://www.isbs2015.gazi.edu.tr/belgeler/bildir
iler/407-411.pdf>
[19] Okeyinka O.M., Oloke D.A., Khatib J.M.
(2016) Salient Parameters Influencing the
Strength Properties of Cement-Less Wastepaper
Based Lightweight Block. Fourth International
Conference on Sustainable Construction
Materials and Technologies (SCMT4) [online].
University of Nevada, Nevada, Las Vegas 7-11
August. Available at: <
http://www.claisse.info/2016%20papers/S147.p
df >.
[20] Roy, R.K., 1990. A Primer on the Taguchi
Method. Van Nostrand Reinhold, New York,
pp.100-154.
[21] Montgomery D.C., (2013) Design and
Analysis of Experiments, John Wiley &Sons,
Inc., 2013
[22] Nuruddin M.F., Bayuaji R.(2009)
Application of Taguchi’s approach in the
optimization of mix proportion for Microwave
Incinerated Rice Husk Ash Foamed Concrete.
International Journal of Civil & Environmental
Engineering IJCEE: Vol 9 (9) pp.121-129
[23] Davies R., Coole T., Osypiw D., (2015), A
review of traditional and Taguchi design of
Experiment: devising a method selection
criteria, Proceedings of 25th Flexible
Automation and Intelligent Manufacturing,
Wolverhampton, United Kingdom 2015,
pp.308-315.
[24] Zarmai, M., Ekere, N., Oduoza, C. and
Amalu, E. (2016) Optimization of thermo-
mechanical reliability of solder joints in
crystalline silicon solar cell assembly.
Microelectronics Reliability [online], 59 pp.
117-125 .
[25] BSI (2000). BS EN 772-13: Methods of test
for masonry units. Determination of net and
gross dry density of masonry units (except for
natural stone). British Standards Institute.
[26] BSI (2011). BS EN 772-1: Methods of test
for masonry units. Determination of
compressive strength. British Standards
Institute.
[27] BSI (1986). BS EN 1881:1986: Testing
concrete. Recommendations for measurement of
velocity of ultrasonic pulses in concrete, (1986)
British Standards Institute.
[28] BSI (2004). BS EN 12504-4:2004: Testing
concrete. Determination of ultrasonic pulse
velocity, (2004), British Standards Institute.
[29] BSI (2011). BS EN 772-4: Specification for
masonry units. Autoclaved aerated concrete
masonry units. British Standards Institute.
[30] BSI (1975). BS EN 2028: Specification for
precast concrete blocks (1975), British
Standards Institute.
[31] Brooks, J. (2014) Concrete and masonry
movements. [online] Butterworth-Heinemann.
[32] Santamaria J., Fuller B., Fafitis A, (2007)
Structural properties of a new material made of
waste paper. Computational Methods and
Experimental Measurements XIII, WIT
Transactions on Modelling and Simulation, 46,
pp.557-567.
WSEAS TRANSACTIONS on ENVIRONMENT and DEVELOPMENTOkeyinka Oriyomi M.,
Oloke David A., Khatib Jamal M.
E-ISSN: 2224-3496 345 Volume 13, 2017